The Preparation of Transparent Silicone Rubber with Rapid Vulcanization and Ultraviolet Absorbing Effect
International Journal of Materials Science and Applications
Volume 7, Issue 4, July 2018, Pages: 142-146
Received: May 28, 2018;
Accepted: Jul. 23, 2018;
Published: Aug. 17, 2018
Views 649 Downloads 54
Jia Liya, Elkem Silicones Shanghai Co., Ltd., Shanghai, China
Man Zhongbiao, Elkem Silicones Shanghai Co., Ltd., Shanghai, China
Silicone materials have excellent weathering resistance, high and low temperature resistance, anti-yellowing and a series of excellent properties over other materials. In this study vinyl silicone oil as the base polymer, hydrogen silicone oil as a cross-linking agent, vinyl silicone resin and ultraviolet absorber as additives, platinum complex as a catalyst, were used to make ultraviolet absorption of highly transparent silicone rubber. Different structures of silicone resin with vinyl group have different effects on the curing speed of the products. The silicone resin with MMViQ can help achieve rapid curing speed. Due to polarity difference for polysiloxane system and ultraviolet absorber, when necessary a suitable organic solvent may be introduced to increase the compatibility of the ultraviolet absorber with the silicone composition to prepare transparent products. Considering that the addition of organic solvents may have effects such as volatiles and properties, the amount of solvent introduced should be as low as possible. In addition, regarding the amount of the ultraviolet absorber added, too little ultraviolet absorber may not achieve a satisfactory ultraviolet absorption effect, but too much would lead to an increase in the amount of solvent introduced. Different ultraviolet absorber could induce different ultraviolet absorption effect and aging resistance.
The Preparation of Transparent Silicone Rubber with Rapid Vulcanization and Ultraviolet Absorbing Effect, International Journal of Materials Science and Applications.
Vol. 7, No. 4,
2018, pp. 142-146.
N. Ribeiro, J.-A. Yang, H.-B. Wang, Y.-X. Lin, M. Murakami, T. Unezaki, H. Makio, “Polymerizable Composition for Optical Material and Use Thereof,” WO2018070383A1 [P], April 19 2018.
J. Park, J.-H. Bae, J. Jung, D. Kang, “Flexible Liquid Crystal Lens,” US2018107056A1 [P], April 19 2018.
J.-H. Lee, S.-J. Park, S.-H. Hwang, B.-J. Mun, H.-S. Song, “Resin Composition for Optical Material and Optical Film Comprising the Same,” KR20180018334A [P], February 21 2018.
H. Kametani, S. Ogi, K. Imazumi, N. Kiyoyanagi, J. Ichikawa, T. Mizu, guchi, R. Shitara, “(Meth) acrylate Compound, Resin Composition Containing the Same, Cured Product of the Resin Composition, and Energy Ray-Curable Resin Composition for Optical Lens Sheet and Cured Product thereof,”CN101675089A [P], March 17 2010.
J. Wang, X.-H. Zhang, X.-M. Zhang, X.-L. Kong, C.-C. Li, E.-L. Xiao, Q. Zhang; L.-P. Sun, PVC “Composition Used for Fresnel Lens and Preparation Method,” CN102863709A [P], January 09 2013.
T. G. Pett, T. J. Hebrink, N.-Y. Jing, J. A. Riddle, D. S. Thompson, A. K. Hartzell, J.-K. Liu, “Silicone-Based Material,” CN102918093A [P], February 06 2013.
S.-M. Xing, Y.-L. Wang, “Organic Silicone Synthesis Technology and Product Application,” p.717, 2000.
A. Pouchelon, F. Lafaysse, “Method for Obtaining a Fibrous Material/Silicone Composite and Said Fibrous Material/Silicone Composite,” CN101680162 [P], March 24 2010.
M. Bahadur, R. Nelson, M. Strong, “Silicone Composition for Producing Transparent Silicone Materials and Optical Devices,” CN102414275 [P], April 11 2012.
K. Nishijima, T. Iimura, M. Suto, T. Sagawa, H. Furukawa, “Curable Silicone Composition, Cured Product Thereof, And Optical Semiconductor Device,” CN 105518076 [P], April 20 2016.
T. Yamazaki, T. Kashiwagi, M. Wakao, “Addition-Curable Silicone Resin Composition and Die Attach Material for Optical Semiconductor Device,” CN105924974 [P], September 07 2016.
T. Shiobara, T. Kashiwagi, K. Imazawa, “LEDs-Forming Silicone Resin Composition and Silicone Lens,” US7829651 [P], November 09 2010.
K. Miyoshi, “Silicone Resin Composition for LED Devices,” US20040116640 [P], June 17 2004.
L. L Zhang, Z. C. Li, X. Xu, “Ultraviolet-Curable Organic-Silicon Liquid Optical-Adhesive Composition and Preparation Method of Composition,” CN107674640A [P], February 9 2018.
K. Sato, T. Ozai, E. Tabei, “Addition-Curable Silicone Resin Composition, Method for Producing Said Composition, and Optical Semiconductor Device,” TW201734135A [P], October 1 2017.